**Ultrasonic Measurements of the Strip Thickness, Lubricant Film **

**Thickness, Roll Deflection and Roll Stress in the Roll Bite in the Cold **

**Rolling of Steel **

**By: **

### Andrew Kevin Hunter

### A thesis submitted in partial fulfilment of the requirements for the degree of

### Doctor of Philosophy

### The University of Sheffield

### Department of Mechanical Engineering

**Summary **

In cold rolling the interface between the roll and strip, known as the roll bite, is key to the finish and geometry of rolled products. This interface is complex and operates in the mixed regime with part asperity contact and part fluid film. The factors which affect this are of interest to the cold rolling community. The inaccessibility of the interface has made direct measurement of its condition difficult. In this thesis ultrasonic approaches have been developed to measure the state of the roll bite, in-situ and in real time.

The thesis starts by introducing the background theory underpinning modern cold rolling. The theory behind the proposed ultrasonic measurements is developed. It is proposed that the proportion of longitudinal and shear waves reflected by the asperity and lubricant film components of the mixed mode interface are dependent on their respective stiffnesses. From these the lubricant layer thickness can be calculated. It is also shown how time-of-flight measurements can be used to measure strip thickness, roll stress, roll deflection and roll material properties.

Ultrasonic sensor systems were incorporated into pilot and semi-industrial cold-rolling mills. Measurements were taken as steel was rolled under a range of lubrication conditions, with rolling velocities from 25 m/min to 1200 m/min and elongations from 5% to 50%. Stiffness and lubricant film thickness measurements were demonstrated for films from 0.3 Β΅m to ~6 Β΅m. Roll bite contact lengths of 9.13mm to 15.34mm were recorded for elongations from 9.7% to 40%. For these same elongations average radial roll stresses of 180 MPa to 340 MPa and roll deflections of 30 Β΅m to 55 Β΅m at the roll bite centre were measured. Time-of-flight measurements yielded thickness profiles of strip reduced from 2.8mm to 2.154mm.

Validation was provided by multiple numerical models which showed good agreement with the ultrasonic results.

**Acknowledgments **

This thesis is just a small window into a process that has involved many late nights, early starts, successes, failures, moments of inspiration and months of head-scratching. Too many people to mention have helped me throughout this. In particular, it would be remiss of me to not give credit and my thanks to the following:

Firstly Iβd like to thank my supervisor Rob Dwyer-Joyce for all his support and advice. It has been a genuine pleasure working under your guidance and I look forward to continuing working with you in the future. Thanks to everyone at the Leonardo Centre for Tribology who has assisted me directly and indirectly, especially Robin Mills and Dave Butcher for his technical wizardry. I gratefully acknowledge the funding received from the European program RFCS (Research Fund for Coal and Steel) which enabled this research. Thanks to the whole Rollgap project team, it was a pleasure working with you. Specific thanks must go to Nicolas Legrand and Nathalie Labbe at Arcelor Mittal for all your support.

Thanks to Phil Harper. Phil I would not have had this opportunity were it not for you and Iβm lucky to consider you both a mentor and a friend. Also thanks to the rest of the team at Tribosonics Ltd. and particularly Tapiwa Mutasa for his perspective on many problems.

Thanks to Yves Carretta at the University of LiΓ¨ge for his advice and computational modelling work.

Thanks to all my friends with a special mention to Henry Brunskill, Iβve never met anyone with such boundless infectious energy, and to Oscar for his endless humour.

My love and thanks to all my family for your support throughout the years, my Grandma, my brothers, James and Michael, and my Dad. I finally finished it!

And last, but not least, my wife Keeley. Thank you for the endless support, patience, love and care you have given me. I love you.

**Table of Contents **

Summary ... i

Acknowledgments ... ii

Table of Contents ... iii

Nomenclature ... vi

Abbreviations ... x

1 Introduction ... 1

1.1 The Development of Rolling ... 1

1.2 Rolling Today ... 4

1.3 Modern Rolling Mills ... 6

1.4 Nature of the Problem ... 7

1.5 Proposed Solution... 9

1.6 Aims ... 9

1.7 Benefits ...10

1.8 Layout of Thesis ...11

2 Cold Rolling of Steel ...13

2.1 Mathematical Model Assumptions and Simplifications ...13

2.2 Cold Rolling Model Overview ...14

2.3 Roll Deformation ...19

2.4 Contact Pressure Distribution ...21

2.5 Strip Deformation ...24

2.6 Roll Stress ...34

2.7 Roll Bending ...38

2.8 Rolling Lubricants...39

2.9 Existing Roll Bite Measurement Techniques ...42

2.10 Conclusions...45

3 Ultrasonic Waves in Elastic Media ...47

3.1 Definition of Ultrasound ...47

3.2 Ultrasonic Wave Basics ...47

3.3 Ultrasonic Wave Equations ...53

3.4 Thin Film Measurement Techniques ...58

3.5 Reflections from an Embedded Layer ...60

3.6 Conclusions...69 4 Acoustoelastic Effect ...71 4.1 Literature Review...71 4.2 Deflection Effect ...72 4.3 Density Effect ...72 4.4 Elasticity Effect ...74 4.5 Time of Flight ...81

4.6 Time of Flight Measurement Techniques ...83

4.7 Stress Induced Refraction ...85

4.8 Acoustoelastic Beam Steering in a Cold-Rolling Contact ...94

4.9 Conclusions...103

5 Ultrasonic Transducers ...105

5.1 Active and Passive Ultrasonics ...105

5.3 Piezoelectric Transducers ... 107

5.4 Piezoelectricity ... 111

5.5 Beam Shape ... 123

5.6 Conclusions ... 129

6 Instrumentation and Experimental Setup ... 130

6.1 Rolling Mills ... 130

6.2 Data Acquisition Equipment ... 133

6.3 Ultrasonic Transducers ... 144

6.4 Strip Material ... 146

6.5 Lubricants and Properties ... 147

6.6 Work Roll Instrumentation ... 151

6.7 Test Conditions ... 166

6.8 Conclusions ... 167

7 Preliminary Testing ... 169

7.1 Thin Film Measurement Techniques ... 169

7.2 Acoustoelastic Constants ... 177

7.3 Cable Length... 183

7.4 Slip Ring Noise ... 185

7.5 Sensor Temperature Dependence ... 187

7.6 Cold Rolling Pilot ... 189

7.7 Conclusions ... 200

8 Ultrasonic Signals, Geometry and Material Properties ... 203

8.1 Ultrasonic Signals ... 203

8.2 Plug Material Properties ... 210

8.3 B-Scans ... 215

8.4 Roll Bite Width ... 223

8.5 Strip Thickness... 229

8.6 Conclusions ... 234

9 Roll Bite Interface Measurements ... 235

9.1 Surface Roughness ... 235

9.2 Ultrasonic Data Capture and Processing ... 236

9.3 Interference Effects ... 241

9.4 Overall Interface Stiffness ... 244

9.5 Shear Interface Stiffness ... 247

9.6 Liquid Stiffness ... 253

9.7 Film Thickness ... 255

9.8 Friction ... 266

9.9 Conclusions ... 270

10 Roll Stress and Deflection ... 271

10.1 Test Conditions ... 271

10.2 Time of Flight Extraction ... 271

10.3 Ultrasonic Data Capture and Processing ... 275

10.4 Deflection and Stress with Rolling Speed ... 277

10.5 Deflection and Stress with Strip Elongation... 286

10.6 Comparison of Elongation and Rolling Speed ... 294

11 Numerical Modelling ...299

11.1 Wave Propagation - PZFlex ...299

11.2 Finite Element - Metafor ...309

11.3 Strip Rolling Model β Metalub ...316

11.4 Conclusions...330

12 Uncertainties, Conclusions and Future Work ...333

12.1 Time-of-Flight Uncertainty ...333

12.2 Amplitude Uncertainty...334

12.3 Film Thickness Model Sensitivity ...340

12.4 Conclusions...345

12.5 Future Work ...352

**Nomenclature **

The following is a list of the characters and symbols used in this thesis. To maintain consistency with naming conventions in some cases the same character has been used to denote more than one parameter, although never within the same chapter. To avoid confusion, the chapter where each parameter has been used has been listed.

**Parameter ****Units ****Chapter Description **

*A * - 2 Proportion of asperity contact

*A * - 3 Wave amplitude

*A * - 3 Apparent area of contact

*AR* - 3 Real area of contact

*ARef* - 7 Reference wave amplitude

### π΄

0 - 3 Initial wave amplitude*a * m 2 Half contact width

π1 m 2 Half contact width of the stick zone

*Ξ± * Nepers/m 3, 8 Attenuation coefficient

*Ξ± * - 4 Acoustoelastic constant

*Ξ± * 1/MPa 9 Pressure-viscosity coefficient

*B * GPa 3 Bulk modulus

*B1, B2, B3* - 8 First, second and third reflection numbers

*b * - 2 Simplifying factor defined in Equation 2.66

*π½ * rad 2 Angular position of element

*C * - 2 Constant of integration

*C * pF/m 6 Cable capacitance

*c * m 2 Half width of roll support bearing

*c * m/s 3 Speed of sound

*cL, cS, *π_{π
} m/s 3 Longitudinal, shear and Rayleigh wave speed of sound

*c1, c2* m/s 3 Speed of sound in the materials either side of an
interface

ππΏππβπ‘ m/s 6 Speed of light in a vacuum (=2.9979x108m/s).

*D * m 2 Roll diameter

*D * m 5 Diameter of the piezoelectric element

π0 m 4 Initial length

*d * - 2 Draft or reduction

*d * C/N 5 Piezoelectric charge constant

*df* m 5 Diameter of the sensing spot

*β * m 2 Roll deflection

βπ Hz 8 Fast Fourier transform frequency step

βπ‘π, βπ‘πΏ, βπ‘πΈ s 4 Change in time of flight due to density, deflection and

elasticity

πΏ m 4 Deflection

*E * Pa 2, 3 Youngβs modulus

*ER, ES* Pa 2 Youngβs modulus of the roll and strip

*el% * % 2 Elongation percentage

π - 2 Stick-slip ratio

π0 F/m 5 Permittivity of free space (= 8.85x10-12 F/m)

πΜ ππ - 11 Equivalent plastic strain

ππ - 5 Relative permittivity

ππ₯*, π*π¦*, π*π§ - 4 Strain in x, y, z directions

*F * N 2 Roll Normal Force

πΉπ N 2 Contribution to horizontal force made by the radial

pressure

*FR* N 2 Radial force applied by the roll

πΉπ N 2 Contribution to horizontal force made by a shear

stress

*Fz* m 5 Transducer focal zone

*f * N/m 2 Specific rolling force

*f * Hz 3 Wave frequency

*fm* Hz 3 Resonant frequency of liquid layer

ππ Hz 8 Sampling frequency

*G * Pa 2, 3 Shear modulus

*g * Vm/N 5 Piezoelectric voltage constant

ππ₯, ππ§ m2/s 4 Gradient of speed of sound array

*H * - 2 Simplifying factor defined in Equation 2.76

*h * m 2 Strip thickness

*h * m 3 Fluid layer thickness

*h0, h1* m 2 Entry and exit strip thickness

βπ m 9 Inlet film thickness

*K * N/m2 _{3 } _{Liquid layer stiffness per unit area }

πΎ`πΏ*, πΎ*`π N/m2 3 Longitudinal and shear stiffness of interface

πΎπ*, πΎ*π N/m2 3 Normal and shear stiffness of interface

*k * N/m 3 Spring constant

*k * HzΒ·s/m 3 Wave number

*k * - 5 Electromechanical coupling factor

*k * - 6 Dielectric constant of cable insulator

*k * Pa 11 Yield shear stress

*L * m 2 Roll bite contact length

*L * ΞΌH/m 6 Cable inductance

*L0, L1* m 2 Strip lengths before and after rolling

*Ly* m 2 Centre to centre distance between the roll bearings

l GPa 4 Third order elastic constant

l m 6 Cable length

l s 8 Pulse length

*Ξ» * m 3 Wavelength

*Ξ» * GPa 4 Second order elastic constant

*m * kg 3 Mass

*m * - 3 Mode of resonance

m GPa 4 Third order elastic constant

*ΞΌ * - 2 Friction coefficient

*ΞΌ * - 4 Second order elastic constant

π0 H/m 6 Permeability of free space (=4Οx10-7 H/m)

ππΆ*, π*π - 11 Coulomb and Tresca friction coefficients

*ΞΌm* - 2 Minimum coefficient of friction

*N * HzΒ·m 5 Frequency constant

*N * m 5 Nearfield distance

*N * - 8 Number of samples

*N * - 12 Number of averages

*n * - 3 Ratio of acoustic impedances as defined in Equation
3.79

*n * GPa 4 Third order elastic constant

*n * - 8 Number of pulse cycles

π0 mPaΒ·s 9 Viscosity at ambient pressure

ππ mPaΒ·s 11 Viscosity at the glass transition temperature

π Hz 3 Angular frequency

π0 - 3 Simplification as defined in Equation 3.14

ππΌ, ππ , ππ Pa 3 Incident, reflected and transmitted wave pressures

ππ Pa 3 Wave pressure

ππ N 2 Radial roll force

*p * Pa 2 Normal pressure

*pR* Pa 2 Radial pressure applied by the roll

ππππ₯ Pa 2 Maximum pressure

πππππ Pa 2 Mean interface normal pressure

π0 rad 3 Phase angle

Q C 5 Piezoelectric charge

ππ - 5 Mechanical quality factor

*q * Pa 2 Interface tangential stress

*R * - 3 Reflection coefficient

*R * m 2 Roll radius

*R * m 5 Distance from the transducer

*Rβ * m 2 Deformed roll radius

*Rp* Hz 8 Pulse repetition rate

*Ra, Rq, * ΞΌm 3 Roughness parameters

ππ ππ ΞΌm 3 Root mean square roughness

π kg/m3 _{3 } _{Density }

ππ % 4 Forward slip

s - 2 Symbolic variable giving the position from the centre of the contact

s m2_{/N } _{5 } _{Elastic compliance }

*π * Pa 2 Compressive stress

π - 12 Standard deviation

π1*, π*2* * Pa 2 Tension at entry and exit to roll bite

πππΈ - 12 Standard error

π1,π₯π§ Pa 2 Principal stress 1

π2,π₯π§ Pa 2 Principal stress 2

ππππ₯ Pa 2 Maximum stress

ππππ Pa 2 Minimum roll pressure

ππ¦ππππ Pa 2 Tensile yield stress

*T * o_{C } _{6 } _{Temperature }

*T * - 3 Transmission coefficient

*T0* s 3 Time period of wave

*Tg* oC 11 Glass transition temperature

*tan(Ξ΄) * - 5 Dielectric loss factor

π‘π s 8 Excitation pulse width

*Οl* Pa 2 Interface shear stress

*Οa, Οl* Pa 2 Shear stress, asperity and lubricant components
*π * rad 2 Angle dependant on position in roll bite

π1*, π*2* * rad 3 Angle of incidence and refraction

ππ rad 2 Angular position of the neutral point

U J 4 Strain energy

u m 3 Spring extension

*V * m3 _{3 } _{Lubricant volume }

*vI, vR, vT* m/s 3 Incident, reflected and transmitted wave particles

*vin, vout* m/s 2 Entry and exit strip velocities

*vr, vs* m/s 2 Roll and strip velocities

*Ξ½ * - 2 Poissonβs ratio

*Ξ½R, Ξ½S* - 2 Poissonβs ratio of the roll and strip

π£πΉπππ‘ππ - 6 Velocity as a percentage of the speed of light in a

vacuum

*W * m 2 Strip width

*w * - 2 Simplifying factor defined in Equation 2.67

*x * m 2 Distance along roll bite

ππΆππππ Ξ© 6 Cable electrical impedance

*z * m 2 Vertical distance from centre of strip

**Abbreviations **

The following is a list of abbreviated terms used within this thesis:
*ADC * Analogue to Digital Convertor

*COTS * Commercial Off The Shelf
*DA * Direct Application
DC Direct Current

EHD/EHL ElastoHydrodynamic Lubrication

EM ElectroMagnetic

*EMAT * ElectroMagnetic Acoustic Transducers
*EMI * ElectroMagnetic Interference

*FFT * Fast Fourier Transform
*LSB * Least Significant Bit

*MPH * Micro-Plasto-Hydrodynamic Lubrication
*mpm * Metres Per Minute

*Mtpa * Million Tons Per Annum
*NDT * Non-Destructive Testing

*PCI * Peripheral Component Interconnect
PHD PlastoHydrodynamic Lubrication
Pk to Pk Peak to Peak Amplitude

PRF/PRR Pulse Repetition Rate/Pulse Repetition Frequency
*PZT * Lead Zirconate Titanate

RE Recirculated (lubricant) RPM Revolutions Per Minute SNR Signal to Noise Ratio

*SoS * Speed Of Sound

*TOEC * Third Order Elastic Constant
*ToF * Time of Flight

**1 Introduction **

This thesis is concerned with ultrasonic measurements in cold metal rolling. The work presented builds on a range of previous research and aims to extend this in a number of areas. To give the work presented herein any meaning it is first important to understand the context in which the work is undertaken and foundations on which it builds. The following chapter aims to populate this back-story by giving an introduction to the topic of rolling, the historical context of the research put forward, the nature of the problem being researched and an overview of the aims, benefits and layout of the thesis.

**1.1 The Development of Rolling **

It is impossible to accurately identify a single inventor of the rolling mill. Like so many inventions
the first rolling mill designs for which records exist were sketched by Leonardo da Vinci. These
*can be found in the Codex Atlanticus and Paris Manuscript I. The sketch in the Paris manuscript, *
as shown in Figure 1.1, is dated between 1497 and 1505. This shows sheet rolling with backup
rolls. There is no evidence that these designs were ever built and it is believed that small hand
driven rolls were used prior to this to flatten gold and silver for the manufacture of jewellery
(Eppelsheimer, 1938).

**Figure 1.1: Rolling Mill designs sketch by Leonardo da Vinci, showing Sheet Rolling with Backup **
Rolls (Leonardo da Vinci, 1488β1505).

Metal rolling did not begin to gain particular significance until the end of the 16th_{ century when }
a slitting mill was setup in Dartford, Kent by Godefroi de Bochs under a patent granted in 1588
to Bevis Bulmer (Tyson, 1996). The mill was powered by waterwheel and cut iron, which at the
time was only available in plate form, for nail production (How, 2015). Similar mills in Germany

and Belgium were being developed around the same time. These were designed for use with softer metals, predominantly lead being produced for roofing, flashing and guttering (Roberts W. L., 1978).

The rolling of iron probably originated in Great Britain around the middle of the 17th_{ century and }
it is known that in 1665 a rolling mill was in operation in the Parish of Bitton, near Bristol, that
was used to roll iron into thin flats (Mackintosh-Hemphill, 1953). By 1682 water-driven rolling
mills for ferrous metals were in operation at Swalwell and Winlaton, near Newcastle.

Over the next century rolling mill design gradually progressed with the introduction of various grooved rolls, rolling tables and reversing systems until in 1783 when William Playfield submitted a patent for a two-high single stand rolling mill that had a similar form to modern rolling mills, as shown in Figure 1.2 (Mackintosh-Hemphill, 1953).

**Figure 1.2: Two-high single stand mill design from William Playfieldβs 1783 patent (Roberts W. **
L., 1978).

In 1779, the Royal Navy's victualling commissioners approached noted ironmaster Henry Cort, offering him a contract to produce iron hoops for their barrels. Apart from supplying new hoops, the contract obliged Cort to convert old hoops into new at the rate of two tons old, to one ton new. Cort built a rolling mill at Fontley and began experimenting with grooved rollers instead of hammering to make the new hoops. In 1783 Cort patented this process which promised a possible eight-fold increase in the capacity of an average charcoal forge. Figure 1.3 shows a sketch of how such an ironworks would have looked, including a grooved rolling mill. The processes patented by Cort are credited with revolutionising iron production in Britain, paving the way for the cheap railway lines and the wire used in electric telegraphs which spurred on the industrial revolution (Eley, 2012).

In the 1780βs the power source for industrial machinery began shifting from water power to steam engines. It is known that around this time John Wilkinson employed a Boulton and Watt steam engine to power, amongst other machinery, a rolling and slitting mill at his Bradley Works (Davis, 1987).

Successive stands (sets of rollers) were introduced by James Cockshutt and Richard Crawshay in a four-high tandem mill near Sheffield in around 1790, the top and bottom rolls of which were driven by separate weighted waterwheels that also acted as flywheels (Roberts W. L., 1978).

**Figure 1.3: A sketch of an Ironworks typical of the early 19**th_{ century showing a water-wheel }
driven grooved rolling mill (Annandale, 1894).

A patent issued to Sir Henry Bessemer in 1857 which described the casting of metal between rollers, was the precursor to contemporary continuous hot mills. Bessemerβs original sketch is shown in Figure 1.4. J.T. Newton of Ystalyfeva, Wales was issued a patent describing the predecessor to the modern cluster mill in 1862.

**Figure 1.4: Sir Henry Bessemerβs original sketch showing twin-roll casting of metals (KMM **
Metals, n.d.).

**1.2 Rolling Today **

Today greater tonnages of metals are processed by rolling than by any other technique (Roberts
W. L., 1978). Approximately 40% of steel production goes to flat rolled products. As of 2007 this
equated to approximately 480 Mtpa (million tons per annum) worldwide (Capital Market Days
2007, 2007). One estimate from 2012 put the revenue from flat rolled steel products as $7.3
billion in the US market alone (Steel Rolling & Drawing in the US: Market Research Report, 2012).
Rolling is just one in the long chain of processes that form the steel industry value chain. Industry
*terminology often categorises these processes as Upstream which includes the production of *
*iron and steel, and Downstream processes which cover the production of semi-finished products *
like blooms, billets, slabs and ingots as well as finished plate and foil products. Figure 1.5 shows
a typical chain of processes (SSAB Sheet Steel, n.d.), starting with the output from the steel
manufacture. The actual set of methods used will depend on the requirements of the final
product.

*Within the industry a distinction is often made between long and flat products. Long products *
*such as structural beams are rolled from rectangular section blooms, and smaller bars, rods and *
*wires are rolled from square section billets. These products are most commonly used in civil and *
structural applications. Flat products such as plates and coiled sheets are rolled from flat
*cross-section slabs. Automotive and appliance manufacturers are the largest consumers of flat *
products (C. Egenhofer, 17 December 2013).

*There are two key categories of rolling: Hot Rolling and Cold Rolling. Hot rolling is performed on *
a metal which has been heated to above its recrystallisation temperature, for steel this is around
920Β°C (Hot Rolled Vs. Cold Rolled Steel, n.d.). Hot rolling can be used to alter the as-cast structure
of the material. During rolling the original grains change shape and careful control of the hot
rolling variables can be used to control the resultant microstructure. Large deformations of the
metal can be made when hot rolling. A primary drawback of rolling at these temperatures is the
tendency for the strip to oxidise, causing the formation of surface iron oxide layers known as
*mill scale (United States Steel Corporation, Association of Iron and Steel Engineers, 1985). This *
is detrimental to the surface finish, coating ability and corrosion resistance of the rolled product.
For these reasons hot rolling is predominantly used to manipulate material geometry rather
than achieving precise surface finish and mechanical properties.

The alternative to hot-rolling is cold-rolling which is performed on metal that is below its recrystallisation temperature, typically at ambient. This generates dislocations in the metalβs crystal structure. These dislocations resist further slip, resulting in work hardening of the metal. Cold rolling can therefore be used to alter the microstructure of the metal, adding strength. Also a more accurate thickness and smoother surface finish can be achieved in comparison to hot rolling. The hardening effects of Cold Rolling can cause the strip to become brittle and hard. Cold rolled strip is therefore often annealed to restore some formability to the strip (SSAB Sheet Steel, n.d.). Cold rolled sheet can be further processed by coating to provide protection against corrosion. For steel, hot-dip zinc galvanizing is one of the most common methods. Other widely used methods include, tin coating, chromium coating, aluminising and Terne coating (a mixture of 80% lead and 20% tin) (C. Egenhofer, 17 December 2013). Coated products may also be painted to further prevent corrosion. This is ineffective with hot rolled products due to scaling (EPA Office of Compliance, 1995).

**Figure 1.5: Typical Flat Steel Product Production Processes (SSAB Sheet Steel, n.d.). **
A large part of the cost of producing flat steel product is its transportation. Another large
contributor is the cost of energy (C. Egenhofer, 17 December 2013). Many of the processes in
the chain are energy intensive, especially those that require elevated temperatures such as steel
production, hot rolling and annealing. To reduce these costs and for practical reasons, such as
the availability of power and transport links, the various processes are often integrated into one

plant. Plants are laid out based upon the material flow through the factory, and as such are often linear. For larger plants shipping is the only practical way to transport the quantity of steel produced and so these plants often incorporate, or are located near to, a port. It is normally only economical to build integrated plants which produce 2 Mtpa or more. Currently the largest integrated steel plant is located in Gwangyang, South Korea and is owned and operated by POSCO (formerly Pohang Iron and Steel Company). Gwangyang Steel works produced 19.5 million tons of crude steel in 2010 (POSCO, n.d.).

**1.3 Modern Rolling Mills **

Although the scale and complexity of rolling mills has evolved over time, their basic principles remain the same. The setup of a rolling mill will vary dependent upon the processing it is required to do. The yield, initial strip thickness, thickness reduction, rolling speed, surface finish, rolling force and required work hardening will all have an influence on the design used.

Despite this all modern rolling mills share a set of similar features and terminology. Figure 1.6 shows a schematic of the key components of a modern mill. It can be seen that the basic principle of the machine is fairly straightforward, however modern rolling mills are complex mechanisms which incorporate a plethora of measurement and control systems. As well as controlling the settings for the mill itself, it is also necessary to coordinate the lubricant delivery, strip tension and the uncoiler/coiler mechanisms.

**Figure 1.6: Schematic of a Modern Rolling Mill **

Figure 1.7 shows a selection of some of the most common roll arrangements used in rolling mills.
*The most basic configuration are 2-High mills, these are often small workshop mills. The rolling *
forces seen in larger mills tend to bend the work rolls resulting in inconsistent strip thickness.
Therefore, backup rolls are used to support the main work roll and maintain its shape. The

*purpose of the 4-High and Cluster variants shown is to reduce the work roll deflection. 3-High *
*mills also achieve this by rolling two strips (or the same strip twice) at the same time. Reversing *
*Mills are those which can operate in either direction, often passing the same piece of strip back *
*and forth through the rolls, gradually reducing the strip thickness in several Passes. The *
advantage of this is that only one stand is required to produce a large elongation of the strip.
However, both the length of strip and throughput are limited. For cases where long strip lengths,
or large throughputs, are required, the strip reduction might be separated out into a number of
*successive roll stands, this is known as a Tandem mill. *

**Figure 1.7: Rolling Mill Configurations **

When multiple stands are used, these need to be synchronised. A change in reduction on one stand will alter the outgoing strip speed and therefore the incoming strip speed to the next stand. This adds yet another degree of complexity to the rolling mill control system. Greater detail on the specifics of the cold rolling mills used in this work are given in later chapters

**1.4 Nature of the Problem **

There is a constant drive for higher quality rolled strip. Aspects of specific interest are strip
thickness, strip flatness and a strip surface free from defects. This drive is intensified due to the
trend of modern rolling mills to combine higher rolling speeds, larger reductions, harder steel
grades and thinner strip. In order to achieve higher product quality, and productivity, it is
**necessary to have a better understanding of the interaction between the strip and work roll **
surface in the roll bite, including an understanding of the friction, heat transfer and lubrication
in the roll gap.

One area in which this greater understanding will help to contribute to improved product, are the preset and adaptation mathematical models used to setup rolling mills. Preset models are

used to determine the initial settings of a mill for a given rolling regime, including entry and exit
strip thickness, rolling speed, entry, exit and intermediate tensions, rolling force, roll gap
**position, rolling torque, flatness actuators and cooling (F. Feldmann, 2009). Friction and heat **
transfers, both into and from the rolls, are two main input parameters for mill preset models.
Current mill presets have poor performance due to the bad estimation of these two parameters.
Poor estimation of these, and inability to measure them accurately in real-time has a knock-on
effect on adaption models. These are the models used to adapt the initial mill settings during
rolling for drift and inaccuracies, specifically in friction, heat transfer and rheology.

Mill preset models are actually made up of a number of sub-models covering tension, speed, roll gap, strip and roll temperature, roll thermal expansion, flatness, roll gap position and sensitivity of outputs to inputs (F. Feldmann, 2009). Most of these relationships are well understood and measured in modern mills, however while work has been completed to theoretically model the roll bite (Ford, Ellis, & Bland, 1951), the harsh conditions mean that little empirical evidence has been obtained.

Explaining rolling force and forward slip behaviours against rolling parameters (rolling speed, lubrication, roll roughness etc) has been a major question in modern rolling. Two main factors are considered as responsible for the observed behaviours, friction and strip rheology. Friction is typically considered using the friction coefficient of the Coulomb model. This describes a range of tribological phenomena related to lubrication, speed, temperature etc. However classic Coulomb or Tresca friction laws are over-simplified to describe the complex lubrication regimes present at the interface. Advanced mixed lubrication models have been developed recently to describe these lubrication regimes in cold rolling (Wilson & Sheu, Real Area of Contact and Boundary Friction in Metal Forming, 1988) (Wilson & Chang, Low Speed Mixed Lubrication of Bulk Metal Forming Processes, 1996) (Kosasih & Tieu, 2007). Again experimental data is missing to validate these models.

Inadequate friction conditions can lead to greater surface roughness, especially when
lubrication reaches the hydrodynamic regime, and skidding where the work roll speed is higher
than the strip speed. As well as degradation of surface finish, skidding can also result in
uncontrolled vibrations in the mill stand leading to inconsistent strip thickness and strip breaks.
Other surface defects, such as heat streaks resulting from thermal breakdown of lubricant film
**can also be an issue. **

With friction of clear importance in the rolling process, metal rolling lubricants have a significant impact not just upon the product quality but also energy consumption and roll lifetime. The lubricant must therefore be matched to the rolling conditions. Without knowledge of how the lubrication conditions are affected by rolling force, speed, lubricant composition, reduction and strip tension the correct selection of lubricant and flow rate to match rolling conditions is difficult. Currently these variables are selected using a heuristic approach and adjusted by the mill operator, this leads to inefficiencies and inconsistencies on the process.

The issues mentioned so far relate equally well to both hot and cold rolling. Although this thesis is concerned primarily with the cold case, there is a large cross-over between the two processes and therefore some consideration should also be given to the issues seen in hot rolling. In hot rolling the friction level in the roll bite and wear of the work rolls can lead to rolled-in-scale on the strip surface. There is currently no reliable online indicator or effective industrial

**practice to prevent rolled-in-scale in hot rolling. Consequently, rolled-in-scale, not detected at **
the hot strip mill, is generally revealed on the subsequent pickling process where it is extremely
difficult to remove. This gives rise to unacceptable surface defects and loss of product.

Modelling of hot rolling lubrication is much less advanced than in cold rolling. Therefore, prior to the development of a hot rolling lubrication model, a local friction and lubricant thickness measurement could be a useful to better understand lubrication regimes specific to hot rolling.

**1.5 Proposed Solution **

In cold rolling, the thin film of lubricant existing between roll and strip is clearly crucial to the quality of rolled product, as described above. The roll operates in boundary lubrication, and currently, the film thickness or the amount of asperity contact is experimentally unknown in rolling processes. Roll stress has been measured by means of strain gauges, however this often requires significant modification of the roll to ensure the measured part deforms in a specified manner. Similarly, a number of studies have measured rolling friction, however this often required modification of the rolling surface itself, deeming most such techniques unsuitable for industrial use.

A wealth of previous works have used ultrasonic techniques to measure the lubricant films (Dwyer-Joyce, Drinkwater, & Donohoe, The Measurement of Lubricant Film Thickness using Ultrasound, 2003) in a range of components, specifically piston rings (Harper, Dwyer-Joyce, SjΓΆdin, & Olofsson, 2004), thrust pads (Dwyer-Joyce, Harper, Pritchard, & Drinkwater, 2006), hydrodynamic bearings (Dwyer-Joyce, Harper, & Drinkwater, A Method for the Measurement of Hydrodynamic Oil Films using Ultrasonic Reflection, 2004), EHL contacts (Dwyer-Joyce, Reddyhoff, & Zhu, Ultrasonic measurement for Film Thicknessand Solid Contact in Elastohydrodynamic Lubrication, 2011) and mechanical seals (Anderson, Salant, & Jarzynski, 1999) (Reddyhoff, Dwyer-Joyce, & Harper, A New Approach for the Measurement of Film Thickness in Liquid Face Seals, 2006). This thesis proposes the use of similar techniques to study the lubrication conditions in the roll-bite and stress conditions within the roll. If these techniques can successfully be applied it will allow measurements to be performed without the need to alter the rolling surface, ensuring the measurement process has minimal effect on the rolling process, and strip surface finish.

**1.6 Aims **

This thesis intends to develop an innovative approach, based upon ultrasonic reflection, to measure a number of roll gap parameters in situ. To achieve this the following aims have been set:

1. Develop the concept and underlying theory for a lubrication sensor based on reflected ultrasound. The proposed measurements will rely on the interaction of ultrasound with the system being studied. It is essential that a theoretical model for this interaction is developed so that the measured ultrasonic response can be linked to the associated lubrication condition.

2. Design and implementation of an in situ ultrasonic sensor to carry out measurements stated in the thesis aims. Different sensor designs are to be evaluated and compared in cold rolling conditions using laboratory, pilot and industrial mill tests. Various methods of sensor instrumentation are to be trialled. A successful design will be selected and tested

3. Design of data acquisition system to capture the required data in real-time. This must take into account the required acquisition rates and resolutions, as well as the implementation of real-time processing algorithms and data storage

4. Measurement of oil film thickness and asperity contact in situ. The oil film thickness for a range of cases will be recorded.

5. Measurement of roll stress in-situ. From this roll stress measurement rolling friction will also indirectly be obtained, based upon the relationship between roll stress and friction. 6. Measurement of strip thickness in-situ. Although other proven methods are available to measure strip thickness many of these happen externally to the roll bite. A by-product of the data captured for the other measurements taken is likely to be the ability to measure strip thickness in real-time in the roll bite.

7. The verification of the results obtained from testing by comparison with computer simulations

**1.7 Benefits **

The proposed work should contribute to the following direct industrial benefits, and wider benefits to society:

1. Improved strip thickness through better mill presets: Existing models for roll force calculation will be considerably improved through the data gained from the proposed sensor.

2. Decreasing strip surface defects: Currently, rolled-in-scale losses are estimated to Β£470k per year for one hot strip mill of 4 Mtpa. Assuming that 3% of rolled-in scale defects appearances could be avoided by the improved models obtained with these sensors, and given the annual EU hot coils production of about 80 Mtpa, means a potential saving in the order of Β£350k per year for the European steel industry alone. Similar benefits also exist in cold rolling.

3. Selecting roll steel grades: The criteria used by roll suppliers for roll steel grades selection and treatment are dependent on the temperature and stress in the contact and the relative motion between the strip and roll. The sensor should define these criteria more accurately.

4. Improve mill productivity by minimising roll degradation: A much better understanding of the interaction between the different roll damage mechanisms (fatigue, oxidation, abrasion) will generate more predictive fatigue and wear models that will decrease the problem. Currently, roll degradation generates losses estimated to Β£3.9M per year on a hot strip mill of 4 Mtpa. Extended across Europe this amounts to around Β£78M per year. If the sensor developed in this thesis contributes a decrease of 3% to these losses, benefits of about Β£2.3M per year can be expected in Europe alone.

5. Competitiveness: With the above industrial benefits, the competitiveness of the steel rolling sector should be increased as the productivity, quality of rolled products, and life of work rolls will be improved. Note that steel producers, roll suppliers and mill automation systems suppliers shall benefit from these advanced sensors by increasing their expertise.

6. Positive impact on occupational health, safety, and working conditions: The integrated sensors, through the better understanding of the roll bite phenomena, will minimise rolled strip quality defects and will avoid many critical situations such as strip breaks due

to bad friction conditions. A positive impact can therefore be expected on working conditions.

7. Preservation of natural resources, energy and environment: The sensor, by enabling a better understanding of roll bite phenomena and their use on industrial mills, will decrease roll and strip surface degradation as well as increase strip thickness accuracy. This should directly reduce material losses. Additionally, more effective and efficient use of rolling lubricant will hopefully result in a reduction of the amount required.

**1.8 Layout of Thesis **

This thesis is split into twelve chapters. Although successive chapters build on concepts in previous chapters, they are broadly self-contained. Each chapter aims to detail one aspect of the work completed.

This chapter offers an introduction to the thesis. Following on from this, chapters 2 to 4 cover various aspects of the underlying theory used throughout the thesis. The transducers, instrumentation, experimental design are covered in chapters 5 and 6. Results from preliminary testing performed to verify the proposed techniques and experimental setup are presented in chapter 7. The primary testing and results are shown in chapters 8 through 10, and the computer modelling validation work is detailed in chapter 11. The conclusions of this work and suggestions for future work are included in the final chapter. Referenced works are included at the end of the thesis.

**2 Cold Rolling of Steel **

This thesis sits at the intersection of three distinct areas of study, cold-rolling, ultrasonics and tribology. This chapter presents the fundamental theory behind the cold-rolling and related tribological aspects of the work. Equation proofs have been presented where they are of particular interest in this thesis, are used in later analysis or have been formulated by the author.

**2.1 Mathematical Model Assumptions and Simplifications **

The rolling process is a complex problem and even basic modelling requires an understanding of the interaction between interface tribology, roll mechanics and strip rheology. A number of assumptions have been made to simplify this analysis and these have been described below. Unless it is stated otherwise the mediums under consideration are assumed to be perfectly homogeneous, isotropic, isothermal and elastic. For simplicity the theoretical work presented only considers a 2 dimensional cross section of the rolls and strip, on the plane perpendicular to the axis of the rolls, the X-Z plane as shown in Figure 2.1.

**Figure 2.1: Axis and Plane Definitions **

This plane is located across the midpoint of the roll, and it is assumed that there is reflective symmetry about this plane in the Y-direction. Spreading of the rolled strip in the Y direction is assumed to be negligible. Where forces are shown in diagrams the positive direction of the force corresponds to the direction of the arrow.

The dimensions of the rolls are large in comparison with the dimensions of the contact area. Therefore the stresses in the region of contact are not significantly dependent upon the shape and support of the rolls far from the contact. It is assumed that the stresses may be calculated

to good approximation by considering the rolls as semi-infinite bodies bounded by a plane surface. A mathematical model of this nature, in which only one boundary exists and all others are infinitely far away, is commonly known as a half-space.

**2.2 Cold Rolling Model Overview **

In its most basic form rolling is used to reduce an input strip to a predetermined thickness, by deformation between two cylindrical rollers. A range of more complex cases exist, such as the use of shaped rolls to create products with a non-uniform cross section, however only simple thickness reduction rolling is considered in this thesis. This reduction can be achieved either with a preheated strip (hot-rolling) or an unheated strip (cold-rolling), as described in the previous chapter. This thesis only considers the cold case, although much of the work is applicable to either.

The energy required to deform the strip can be thought of as coming from four sources, strip
backward tension, strip forward tension, roll force and roll torque, as shown in Figure 2.2. Roll
torque is transmitted to the strip via friction in the roll-strip interface. This interface is referred
*to as the roll bite and the characteristics of this interface strongly influence the effectiveness *
and efficiency of the rolling process. It is common for a lubricant, typically an oil-water emulsion,
to be used in the roll bite for numerous reasons as described towards the end of this chapter.

**Figure 2.2: Primary Forces in Metal Rolling **

As the deformation energy applied by the rolls is transmitted through the roll-strip interface the conditions and interactions here are the predominant interest in this work. To adequately understand this aspect of the system it is also necessary to look into the behaviour in the roll bulk and strip.

**2.2.1 Draft and Elongation **

Large loads are required during rolling to permanently deform the strip, and these can cause elastic deformation of the roll. The roll is flattened and the roll radius local to the contact area

*increases from its nominal value R to its deformed radius Rβ. This slightly increases the roll bite *
*contact length L, shown in Figure 2.3. It also results in stresses inside the roll. Understanding *
these stresses is important for both roll design and condition monitoring.

**Figure 2.3: Roll Schematic **

*As shown in Figure 2.3 the strip thickness is reduced from h0 to h1* the difference between these
*being the draft, d, also referred to as the reduction. *

π = β0β β1 2.1

If we assume conservation of mass and no density change, it must hold that there is no volumetric change. Combining this with the assumption that there is negligible flow of the strip across its width we can state:

β0πΏ0= β1πΏ1 2.2

*Where L0 and L1* are the strip lengths before and after rolling. It is clear that a reduction in strip
thickness results in an elongation of the strip length. It is useful to define this elongation in terms
*of percentage, el%, as given by: *

ππ% = 100πΏ0β πΏ1

πΏ0 2.3

Rolling processes are normally defined by specifying elongation percentage rather than the draft.

**2.2.2 Interface Profile **

The roll bite length, as shown in Figure 2.3, is often of the order of millimetres. It is therefore useful to consider the profile of the roll bite on the microscopic scale. Figure 2.4 shows a schematic of the interfaces and lubricant in and around the roll bite. It can be seen that the contact between the roll and strip is a combination of direct asperity contact interspersed with lubricant filled pockets. This type of contact will be referred to as mixed mode.

Both the lubricant and solid asperity contact contribute to the interface normal pressure and shear stress, in the manner described in Equations 2.4 and 2.5:

π(π₯) = (1 β π΄(π₯))ππ(π₯) + π΄(π₯)ππ(π₯) 2.5

*Where A is the proportion of asperity contact, Ο is the shear stress, p is the normal pressure and *
*the subscripts l and a denote the lubricant and asperity components respectively. The *
proportion of asperity contact is therefore of great importance.

**Figure 2.4: Roll Bite Interface Schematic **

It is also worth noting that, as shown in Figure 2.4 the amplitude of the asperities can be of the same order as the film thickness. Defining a single value for film thickness is therefore non-trivial. In this thesis the surfaces are assumed to have an evenly distributed roughness and the film thickness is taken as the difference between the roughness mean-lines of the two surfaces. Most rolling occurs in the mixed lubrication regime, however at higher rolling speeds hydrodynamic lubrication with a continuous fluid film has been observed, although this rarely happens in practice (Atkins, 1974).

**2.2.3 Roll and Strip Velocities **

If a constant volume of metal is assumed, and no significant spread occurs across the width of the strip, the strip speed must increase relative to the roll surface speed through the roll bite. In normal rolling the incoming strip travels slower than the roll surface while the exiting strip travels at the same speed or marginally faster. This leads to a velocity difference, or slip, between the strip and roll. Part way through the roll bite there is transition point, known as the neutral point, where the slip changes direction. At this point the roll and strip are travelling at the same speed. These various velocities are shown in Figure 2.5.

* Figure 2.5: Roll Bite Velocities, vb and vf* are the backward and forward velocities of the strip

**relative to the roll**

Figure 2.6 shows the velocities of the roll and strip along with the aforementioned neutral point. The location of the neutral point is defined by the friction conditions in the roll bite. Many traditional models of rolling (Atkins, 1974) (Roberts W. L., 1978) put the neutral point near the centre of the roll bite, however in practice it is widely understood that the neutral point is actually nearer to the exit.

**Figure 2.6: Roll and Strip velocity showing the neutral point **

**2.2.4 Interface Friction **

Early models of cold rolling assumed Amontonsβ laws of friction to be applicable, that the ratio of shear to normal stress assumes a constant value along the entire arc of contact and that this ratio is equal to the coefficient of friction. Amontonsβ laws however only apply to dry interfaces and cannot be applied to the lubricated case.

Even later models which account for lubrication assume that this results in a uniform coefficient of friction across the roll bite. However this assumption does not hold true due to the partially hydrodynamic nature of the interface, and non-uniform pressure profile across the roll bite. In hydrodynamic lubrication the frictional effects should be higher at points of highest slip, for example the entry to the roll bite, and will be zero at the neutral point. On the other hand the thickness of the lubricant film is expected to decrease through the roll bite, and this will result in an increasing coefficient of friction due to boundary layer lubrication.

The magnitude of the friction coefficient between the strip and roll affects the relative slip. As the friction coefficient increases backward slip is reduced and the neutral point moves closer to the entry of the roll bite. Conversely as the frictional force is reduced the neutral point will move towards the back of the roll bite. Too little friction and the neutral point will move beyond the end of the roll bite, which results in the roll surface travelling faster than the strip at all points across the roll bite and the rolls skidding. If the frictional forces are too high then positive, or forward, slip occurs (where the strip exit speed is in excess of the roll surface speed) this can result in a poor surface finish and higher energy consumption.

It is therefore desirable to operate as close to the smallest value of friction coefficient before
*skidding occurs, this value is referred to as the minimum coefficient of friction, ΞΌm*. For rolling of
thin strip and foil products this can be as low as 0.01 (Roberts W. L., 1978). Friction is therefore
of great importance to the rolling process. Many mathematical models characterise the roll bite
with a constant coefficient of friction. While this is sufficient for simple analyses it is clear that
this is not the whole story. Lubrication conditions will clearly have a large impact on this.
At the minimum friction level the pressure exerted by the rolls across the contact is essentially
constant. When the coefficient is increased and the neutral point moves into the roll bite a
*friction hill is observed which results in a peak in the pressure exerted by the rolls at the neutral *
point (Seibel, Berichte des Walzwerksausschusses [Reports of the Rolling Mill Committee],
1924), as shown in Figure 2.7. It is worth noting that the rolling force per unit width can be
calculated from the pressure curve by integrating the area underneath it. Various methods of
modelling the pressure distribution are discussed later.

**Figure 2.7: Schematic Illustrating the Hypothetical βFriction Hill" Pressure Distribution along **
**the Arc of Contact **

N e u tra l P o in t E n try P la n e E x it P la n e P re s s u re Distance

Figure 2.8 illustrates that for constant emulsion flow rate, but varying rolling speed, different lubrication regimes occur in the roll bite. For slow speeds the coefficient of friction decreases with speed. The emulsion is behaving like a pure oil and the lubricant is supporting more of the load. However at higher rolling speeds the friction level increases. This is due to the occurrence of starvation.

**Figure 2.8: Stand Speed against Friction for two lubricants, reproduced from Fouratier et al. (A. **
Fouratier, F. GeiΓller, G. Endemann and B. Schmidt;, 2002).

It is clear that rolling is not a simple problem and that any attempt to model it must take into account numerous variables.

**2.3 Roll Deformation **

The deformation of the roll under normal operating conditions is elastic. The elastic deformation of contacting surfaces has been widely studied and much work has been put into mathematically modelling this. Two common approaches, Hitchcock and Hertzian, are presented here.

**2.3.1 Hertzian Approach **

Heinrich Hertz studied the elastic contact of spheres (Hertz, 1896), which was subsequently extended to a range of contacting bodies including a cylinder-on-plate. The cylinder-on-flat contact is treated as a special case of cylinder-on-cylinder contact where the cylinder used to represent the flat is assumed to have an infinite radius (R. G. Budynas, 2011). The cylinder axial lengths are equivalent to the strip width. This gives:

πΏ = 2β2πΉ
ππ
(1 β π_{π
}2_{) πΈ}
π
β + (1 β π_{π}2_{) πΈ}
π
β
1 π·β 2.6

*D is the diameter of roll, E and Ξ½ are the Youngβs Modulus and Poissonβs ratio of material, with *
*the subscripts R and S representing the roll and strip respectively. The pressure distribution is *
*elliptical. Rearranging and substituting for the specific force, f, we get: *

πΏ = 1.596βππ· (1 β ππ 2 πΈπ +1 β ππ 2 πΈπ ) 2.7

This Hertzian approach assumes elastic materials, this is a fair assumption for the roll, however as the strip plastically deforms its validity is questionable. This modelling approach would therefore be much better suited to modelling of the contact between the work roll and backup rolls. A more suitable approach for the roll-strip interface was formulated by Hitchcock (Hitchcock, 1935) who used the elliptical Hertzian pressure distribution to calculate deformed and undeformed roll radii.

**2.3.2 Hitchcockβs Approach **

Hitchcockβs equation for the roll bite length, accounting for a deformed roll is given here:

πΏ =8π
(1 β ππ
2_{)πΜ
}
ππΈπ
+ β[8π
(1 β ππ
2_{)πΜ
}
ππΈπ
]
2
+ π
π 2.8

*Where L is the length of the arc of the deformed contact, R is the undeformed roll radius, Ξ½R* is
*Poissonβs ratio of the roll, ER is Youngβs modulus of the roll, d is the reduction and πΜ
is the mean *
*pressure. The mean pressure is the roll normal force F divided by the contact area, calculated *
*from the roll bite length L and strip width W, as shown in Equation 2.9. *

πΜ = πΉ

πΏπ 2.9

The deformed radius can be obtained from this by the following assumption:

πΏ = βπ β²π 2.10

*Where Rβ is the flattened roll radius. Combining with Equation 2.8 and simplifying to give the *
*relationship in terms of the specific rolling force f, which is the force applied per unit width (π =*
*πΉ/π) gives: *

π
β² _{= π
[1 +}16(1 β ππ
2_{)}

ππΈπ π

π] 2.11

As described at the beginning of this chapter a combination of strip tensions and roll torque, in addition to rolling force, contribute to the deformation of the strip. These are implicit in the reduction term used in Hitchcockβs formula. Hitchcockβs equations have since been shown to under predict the amount of roll deformation and a number of authors have suggested modifications to the equations (Roberts W. L., 1969) and the assumptions made in formulating the equation have been widely criticised (Lenard, 2013). It can be seen from the equation that Hitchcockβs relationship defines the flattened roll shape by a simple radius value, the deformed shape is therefore assumed to be circular. Empirical evidence has shown that the work roll is in fact flattened. This is evident from a basic consideration of the profile as there must be a

transition between the unloaded and deformed profiles at the roll-bite exit and entry. However, Hitchcockβs equation is still widely used as a simple and quick way to estimate both roll flattening and contact length

Figure 2.9 shows a comparison of the roll bite length predicted by the Hitchcock equations.
*Values representative of a real rolling case were used (ER, ES* = 2.1x1011* Pa, Ξ½R, Ξ½S = 0.3, D = 0.4m) *

**Figure 2.9: Contact Length predicted by Hitchcock (Equation 2.8) for a number of reductions **
The mean pressure used in Hitchcockβs equation was calculated from the force and contact
length output from the Hertzian approach. For zero force, Hitchcockβs equation can still be used
to predict contact lengths for non-zero deformations, however clearly no reduction is possible
without a deformation force. Conversely the zero reduction calculation will not hold for
non-zero deformation forces, this has only been plotted in Figure 2.9 to represent the lower bound
of contact lengths predicted by Hitchcockβs formula.

**2.4 Contact Pressure Distribution **

The normal rolling force is the primary mechanism by which strip deformation is achieved. Only by matching the required rolling force to the strip deformation required can an accurate output strip thickness be attained. The preceding analysis allowed for an estimation of contact length, and using knowledge of the normal rolling force which is commonly measured on rolling mills, it is possible to get an estimation for the pressure distribution.

**2.4.1 Stick-Slip Approach **

Two cylindrical rollers of identical material in rolling contact with parallel axis (such that they make a rectangular contact) can be modelled as a plane strain problem with normal and tangential stress distributions at the contacting surfaces (Kalker, 1990).

As described earlier in this chapter there is slip between the surfaces of the roll and strip in cold rolling. This can be modelled by assuming a zone of sticking (zero relative velocity between roll and strip) and a zone of slip (Carter, 1926). This zone can be approximated to a strip shape, and is defined by a stick-slip ratio:

π = π1β π 2.12

*Where ΞΎ is the stick slip ratio, a is half the contact length and a1* is half the contact length of the
stick zone.

**2.4.1.1 Normal Pressure Distribution **

*According to classical contact mechanics the normal pressure distribution, p(x), across the *
*contact zone is elliptical (Johnson, 1987). If the maximum pressure is denoted as pMax* this leads
to the following relationship for the normal pressure distribution, Equation 2.13.

π(π₯) = ππππ₯β(1 β (π₯ πβ )2) 2.13

*Where x is the distance along the roll bite. The half contact width is half the roll bite contact *
length (π = πΏ 2*β ), although for simplicity in later calculations a is retained. Figure 2.10 shows *
the elliptical pressure distribution and equivalent average pressure.

**Figure 2.10: Elliptical Pressure Distribution. **

The integral of these two functions must be equal across the width of the contact; it is therefore
*fairly straightforward to work out the pMax from pMean* using simple geometry to give Equation
2.14.

ππππ₯=

πππππ4

π 2.14

The average pressure is simply the ratio of normal force to contact area, Equation 2.15 πππππ=

πΉ

*Where F is the normal force applied to the rolls and W the width of the contact (strip width). *
Substituting Equation 2.15 into Equation 2.14 along with the force per unit length across the roll
(πΉ = ππ) gives a value for the maximum pressure, Equation 2.16.

ππππ₯ =

2π

ππ 2.16

This can be substituted into Equation 2.13 to give Equation 2.17, the normal pressure distribution across the contact:

π(π₯) =2π
ππβ1 β (
π₯
π)
2
2.17
This is only valid in the contact, where |x| β€ a, outside the contact the normal pressure is zero.
**2.4.1.2 Tangential Stress Distribution **

*In the slip zone the tangential stress q is a function of the normal pressure p and friction *
coefficient π, as shown in Equation 2.18.

π = ππ 2.18

*The tangential stress distribution q(x) over the contact zone is given by (Das Bakshi, Leiro, *
Prakash, & Bhadeshia, 2014):

π(π₯) =
{
0, |π₯| β₯ π
βπ ππ(π )π2π
ππβ1 β (
π₯
π)
2
, βπ β€ π₯ < π β 2ππ
βπ ππ(π )π2π
ππ [β1 β (
π₯
π)
2
β βπ2_{β (π +}π₯
πβ 1)
2
] , π β 2ππ β€ π₯ β€ π
2.19
where
π ππ(π ) = {
+1, π > 0
0, π = 0
β1, π < 0

*Here s is a symbolic variable giving the position from the centre of the contact, as shown later *
in Figure 2.18. The tangential and normal stress distributions where calculated using Equations
2.17 and 2.19. A friction coefficient of ΞΌ=0.3 was used, and the stress was normalised by dividing
*through by the ratio f/a. The results are plotted in Figure 2.11. *

As described in its derivation the normal force distribution is elliptical, and is unaffected by the stick-slip ratio or friction coefficient. The tangential force distribution changes markedly with a change in the stick-slip ratio, as expected from the form of Equation 2.19. The figure also shows that in the slip zone the tangential force is of the same elliptical form as the normal force distribution, but scaled by the friction coefficient.

**Figure 2.11: Normal and Tangential Stress Distribution for a range of ΞΎ, with ΞΌ = 0.3. **

**2.5 Strip Deformation **

The primary purpose of most rolling processes is to reduce the thickness, or alter the cross sectional geometry, of the input material. There are number of other advantages that can be gained by rolling.

Deforming the strip between smooth rollers imprints the surface roughness onto the strip improving the finish. Plastic deformation of the strip induces a residual stress, which is often undesirable. The effect of residual stresses can be decreased by annealing which is used when subsequent processes require the material to have good ductility.

Rolling can also be used to join dissimilar materials in laminates to give improved performance of the final product.

**2.5.1 Strip Flow **

During rolling the strip is deformed in all 3 dimensions. In cold rolling the strip is typically many times wider than it is thick. For this reason, we can assume that the problem is only 2 dimensional, with deformation occurring to the strip thickness and length. While some transverse effects do occur these are concentrated on the outer edges of the strip, so this assumption is appropriate.

In the preceding calculations isothermal conditions are assumed, this implies that all rolling energy is absorbed by the strip and goes into plastic deformation. However, in practice the plastic deformation actually causes some heating of the strip.

Rolling will alter the grain structure of a metal, making it anisotropic, with elongated grains in the direction of rolling. A sketch showing how the strip material flows through the roll bite can be seen in Figure 2.12.

**Figure 2.12: Strip Flow **

Clearly a reduction in strip thickness requires material flow. It is convenient for our analysis to assume that this is entirely plastic, however in reality a certain amount of elastic recovery occurs, as shown in Figure 2.13.

**Figure 2.13: Strip Deformation Zones **

**2.5.2 Strip Deformation Stress **

Assuming no strip tension, the minimum normal pressure that needs to be applied to the strip
to cause deformation is equal to the compressive yield stress. This has been approximated to
1.155 times the tensile yield stress, Οyield (Nadai, The Forces Required for Rolling Steel Strip Under
Tension, 1939). If we take into account the longitudinal stress due to strip tension at the entry
of the roll bite, Ο1*, then the minimum roll pressure Οmin* at the entry of the roll bite is:

ππππ = 1.155ππ¦ππππβ π1 2.20

A similar calculation also applies at the exit of the roll bite.

**2.5.3 Von KΓ‘rmΓ‘n Approach **

One of the most widely used models of pressure distribution was developed by noted aerodynamicist Theodore von KΓ‘rmΓ‘n who used a differential equation to model the pressure along the arc of contact (KΓ‘rmΓ‘n, 1925).The model is based on the equilibrium forces applied to a slab of metal undergoing plastic deformation between two rollers.

The Von KΓ‘rmΓ‘n approach starts by considering a vertical element of the strip between the roll bite entrance and plane of the neutral points (Mukerjee, 1973), as shown in Figure 2.14.

**Figure 2.14: Vertical Strip Element used in Von KΓ‘rmΓ‘n Formulation **

*Where Ο and Ο+dΟ represent the compressive stresses applied to either side of the element. The *
*radial pressure applied by the roll to the strip is pR* at an angle π which is dependent on the
*position of the element in the roll bite. This can be converted to radial roll force PR* simply by
multiplying by the area of the end of the element:

ππ = ππ

ππ₯

cos π 2.21

*The tangential force acting on the end of the element is represented by F. This force can be *
*calculated in terms of pR using the coefficient of friction ΞΌ: *

πΉ = πππ

ππ₯

cos π 2.22

The horizontal components of the forces given in Equations 2.21 and 2.22 respectively are given below:

ππ ,π₯ = ππ tan π ππ₯ 2.23

πΉπ₯ = πππ ππ₯ 2.24

These forces can be balanced with the horizontal forces due to the compressive stresses to give: 2ππ tan π ππ₯ β 2πππ ππ₯ = (π + ππ)(β + πβ) β πβ 2.25

Then by treating the product of the infinitesimal increments as insignificant and using the product rule we can simplify the equation to:

2ππ ππ₯(tan π β π) = π(πβ) 2.26

We can then calculate the vertical components of the forces given in Equations 2.21 and 2.22 respectively:

ππ ,π§ = ππ ππ₯ 2.27

πΉπ§ = πππ tan π ππ₯ 2.28

Equation 2.27 can be substituted into 2.26 to give:

2ππ ,π§(tan π β π) = π(πβ) 2.29

This can be rearranged using the factor rule to give Equation 2.30: ππ ,π§(tan π β π) = π (

πβ

2) 2.30

The vertical force FR,z can be calculated from the vertical pressure p using the following relationship:

ππ ,π§ = ππ

ππ₯

cos πcos π = πππ₯ 2.31

Substituting this into Equation 2.30 gives:

π(tan π β π)ππ₯ = π (πβ

2) 2.32

A similar analysis can be completed for an element between the neutral plane and exit of the roll bite, the only difference being that the direction of the tangential frictional force is reversed, due to the opposite direction of the slip. This results in the following equation:

π(tan π + π)ππ₯ = π (πβ

2) 2.33

Combining Equations 2.32 and 2.33 results in:

π(tan π Β± π)ππ₯ = π (πβ

2) 2.34